LMucko/crystallography-open-database huggingface dataset:
Microwave synthesis and spectroscopic properties of ternary scheelite-type molybdate phosphors NaSrLa(MoO4)3:Er3+,Yb3+
Chang Sung Lim; Aleksandr S. Aleksandrovsky; Maxim S. Molokeev; Aleksandr S. Oreshonkov; Victor V. Atuchin; Journal of Alloys and Compounds 713 (2017) 156–163; doi:10.1016/j.jallcom.2017.04.060

data_1545797
_publ_section_title
;
 Microwave synthesis and spectroscopic properties of ternary
 scheelite-type molybdate phosphors NaSrLa(MoO4)3:Er3+,Yb3+
;
_journal_issue                   0
_journal_name_full               'Journal of Alloys and Compounds'
_journal_page_first              156
_journal_page_last               163
_journal_paper_doi               10.1016/j.jallcom.2017.04.060
_journal_volume                  713
_journal_year                    2017
_chemical_formula_moiety         'Er0.13 La0.93 Mo4 O16 Yb0.27, 1.333(Na Sr)'
_chemical_formula_sum            'Er0.13 La0.93 Mo4 Na1.33 O16 Sr1.33 Yb0.27'
_chemical_formula_weight         985.30
_space_group_IT_number           88
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4ad'
_symmetry_space_group_name_H-M   'I 41/a :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   5.32926(14)
_cell_length_b                   5.32926(14)
_cell_length_c                   11.74788(30)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    300
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     333.652(15)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    64.594
_exptl_crystal_density_diffrn    4.903832
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
no preferred orientation
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        10.392
_pd_proc_ls_prof_wR_expected     13.741
_pd_proc_ls_prof_wR_factor       15.644
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.139
_refine_ls_R_I_factor            2.34
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            NSLM_0p1Er0p2Yb.cif
_cod_data_source_block           a
_cod_original_cell_volume        333.651(20)
_cod_original_sg_symbol_Hall
;
-I 4ad
;
_cod_original_sg_symbol_H-M      I41/a
_cod_original_formula_sum
;
Er0.13 La0.93 Mo4 Na1.33 O16 Sr1.33 Yb0.27
;
_cod_database_code               1545797
Microwave synthesis and spectroscopic properties of ternary scheelite-type molybdate phosphors NaSrLa(MoO4)3:Er3+,Yb3+
Chang Sung Lim; Aleksandr S. Aleksandrovsky; Maxim S. Molokeev; Aleksandr S. Oreshonkov; Victor V. Atuchin; Journal of Alloys and Compounds 713 (2017) 156–163; doi:10.1016/j.jallcom.2017.04.060

data_1545798
_publ_section_title
;
 Microwave synthesis and spectroscopic properties of ternary
 scheelite-type molybdate phosphors NaSrLa(MoO4)3:Er3+,Yb3+
;
_journal_issue                   0
_journal_name_full               'Journal of Alloys and Compounds'
_journal_page_first              156
_journal_page_last               163
_journal_paper_doi               10.1016/j.jallcom.2017.04.060
_journal_volume                  713
_journal_year                    2017
_chemical_formula_moiety         'Er0.07 La0.67 Mo4 O16 Yb0.60, 1.333(Na Sr)'
_chemical_formula_sum            'Er0.07 La0.67 Mo4 Na1.33 O16 Sr1.33 Yb0.6'
_chemical_formula_weight         994.85
_space_group_IT_number           88
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4ad'
_symmetry_space_group_name_H-M   'I 41/a :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   5.30628(10)
_cell_length_b                   5.30628(10)
_cell_length_c                   11.68195(25)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    300
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     328.924(11)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    63.144
_exptl_crystal_density_diffrn    5.022207
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
no preferred orientation
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        9.612
_pd_proc_ls_prof_wR_expected     13.145
_pd_proc_ls_prof_wR_factor       14.634
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.113
_refine_ls_R_I_factor            2.62
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            NSLM_0p05Er0p45Yb.cif
_cod_data_source_block           a
_cod_original_cell_volume        328.924(14)
_cod_original_sg_symbol_Hall
;
-I 4ad
;
_cod_original_sg_symbol_H-M      I41/a
_cod_original_formula_sum
;
Er0.07 La0.67 Mo4 Na1.33 O16 Sr1.33 Yb0.60
;
_cod_database_code               1545798
Crystal chemistry of anion-excess ReO3-related phases II; Crystal structure of PrZr2F11
Laval, J P; Abaouz, A; Journal of Solid State Chemistry 100 (1992) 90–100; doi:10.1016/0022-4596(92)90158-R

data_1545872
_publ_section_title
;
 Crystal chemistry of anion-excess ReO3-related phases II; Crystal
 structure of PrZr2F11
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              90
_journal_page_last               100
_journal_paper_doi               10.1016/0022-4596(92)90158-R
_journal_volume                  100
_journal_year                    1992
_chemical_formula_sum            'F11 Pr Zr2'
_chemical_formula_weight         532.34
_space_group_IT_number           72
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      72
_symmetry_space_group_name_Hall  '-I 2 2c'
_symmetry_space_group_name_H-M   'I b a m'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            4
_cell_length_a                   7.716(4)
_cell_length_b                   10.006(6)
_cell_length_c                   10.897(6)
_cell_volume                     841.3(8)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    8.276
_exptl_crystal_density_diffrn    4.203
_exptl_crystal_F_000             952
_refine_ls_number_parameters     38
_refine_ls_number_reflns         685
_refine_ls_R_factor_gt           0.031
_refine_ls_wR_factor_gt          0.031
_cod_data_source_file            JSSC-1992-100-90-100.cif
_cod_data_source_block           PrZr2F11
_cod_database_code               1545872
Insight into the mechanism of carbon steel corrosion under aerobic and anaerobic conditions
El Mendili, Y.; Abdelouas, A.; Bardeau, J.-F.; Physical Chemistry and Chemical Physics 15 (2013) 9197–9204; doi:10.1039/c3cp50853f

data_7228110
_publ_section_title
;
 Insight into the mechanism of carbon steel corrosion under aerobic and
 anaerobic conditions
;
_journal_issue                   23
_journal_name_full               'Physical Chemistry and Chemical Physics'
_journal_page_first              9197
_journal_page_last               9204
_journal_paper_doi               10.1039/c3cp50853f
_journal_volume                  15
_journal_year                    2013
_chemical_formula_structural     'Fe3 O4'
_chemical_formula_sum            'Fe3 O4'
_chemical_name_mineral           Magnetite
_chemical_name_systematic        'Iron diiron(III) oxide'
_space_group_crystal_system      cubic
_space_group_IT_number           227
_space_group_name_Hall           'F 4d 2 3 -1d'
_space_group_name_H-M_alt        'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.36(1)
_cell_length_b                   8.36(1)
_cell_length_c                   8.36(1)
_cell_volume                     584.3(12)
_exptl_crystal_density_meas      5.2
_cod_data_source_file            YE1.cif
_cod_data_source_block           YE1
_cod_original_cell_volume        575.9
_cod_original_sg_symbol_H-M      'F d -3 m S'
_cod_database_code               7228110
Crystal structure of BaNaZr2F11 : a phase recrystallizing from fluorozirconate glasses
Laval, J. P.; Abaouz, A.; Journal of Solid State Chemistry 101 (1992) 18–25; doi:10.1016/0022-4596(92)90195-2

data_1545878
_publ_section_title
;
 Crystal structure of BaNaZr2F11 : a phase recrystallizing from
 fluorozirconate glasses
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              18
_journal_page_last               25
_journal_paper_doi               10.1016/0022-4596(92)90195-2
_journal_volume                  101
_journal_year                    1992
_chemical_formula_sum            'Ba F11 Na Zr2'
_chemical_formula_weight         551.76
_space_group_IT_number           88
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      88
_symmetry_space_group_name_Hall  '-I 4ad'
_symmetry_space_group_name_H-M   'I 41/a :2'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   8.223(5)
_cell_length_b                   8.223(5)
_cell_length_c                   23.610(14)
_cell_volume                     1596.5(17)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    7.651
_exptl_crystal_density_diffrn    4.590
_exptl_crystal_F_000             1968
_refine_ls_number_parameters     42
_refine_ls_number_reflns         468
_refine_ls_R_factor_gt           0.055
_refine_ls_wR_factor_gt          0.057
_cod_data_source_file            JSSC-1992-101-18-25.cif
_cod_data_source_block           BaNaZr2F11
_cod_original_cell_volume        1597(2)
_cod_original_sg_symbol_H-M      'I 41/a'
_cod_database_code               1545878
Crystal structure of a new oxyfluoride : Tl2Zr3OF12
Mansouri, I.; Avignant, D.; Journal of Solid State Chemistry 51 (1984) 91–99; doi:10.1016/0022-4596(84)90319-0

data_1545882
_publ_section_title
;
 Crystal structure of a new oxyfluoride : Tl2Zr3OF12
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              91
_journal_page_last               99
_journal_paper_doi               10.1016/0022-4596(84)90319-0
_journal_volume                  51
_journal_year                    1984
_chemical_formula_sum            'F12 O Tl2 Zr3'
_chemical_formula_weight         926.42
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                120.
_cell_formula_units_Z            6
_cell_length_a                   7.703(1)
_cell_length_b                   7.703(1)
_cell_length_c                   30.017(2)
_cell_volume                     1542.5(3)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    34.331
_exptl_crystal_density_diffrn    5.984
_exptl_crystal_density_meas      5.940
_exptl_crystal_F_000             2388
_refine_ls_number_reflns         908
_refine_ls_R_factor_gt           0.046
_refine_ls_wR_factor_gt          0.067
_cod_data_source_file            JSSC-1984-51-91-99.cif
_cod_data_source_block           Tl2Zr3OF12
_cod_original_cell_volume        1542.5(5)
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               1545882
Structure du tetrafluorure de zirconium, ZrF4 alpha
Papiernik, R.; Mercurio, D.; Frit, B.; Acta Crystallographica, Section B 38 (1982) 2347–2353; doi:10.1107/S0567740882008760

data_2108041
_publ_section_title
;
 Structure du tetrafluorure de zirconium, ZrF4 alpha
;
_journal_name_full               'Acta Crystallographica, Section B'
_journal_page_first              2347
_journal_page_last               2353
_journal_paper_doi               10.1107/S0567740882008760
_journal_volume                  38
_journal_year                    1982
_chemical_formula_sum            'F4 Zr'
_chemical_formula_weight         167.218
_space_group_IT_number           84
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      84
_symmetry_space_group_name_Hall  '-P 4c'
_symmetry_space_group_name_H-M   'P 42/m'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   7.896(1)
_cell_length_b                   7.896(1)
_cell_length_c                   7.724(1)
_cell_volume                     481.57(11)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    4.4
_exptl_crystal_density_diffrn    4.613
_exptl_crystal_density_meas      4.550
_exptl_crystal_F_000             608
_refine_ls_number_reflns         1335
_refine_ls_R_factor_gt           0.030
_refine_ls_wR_factor_gt          0.031
_cod_data_source_file            Acta-Cryst-1982-B38-2347-2353.cif
_cod_data_source_block           alpha-UF4
_cod_original_cell_volume        481.57(14)
_cod_database_code               2108041
Crystal chemistry of anion-excess ReO3-related phases : crystal structure of beta-PrZr3F15
Laval, J. P.; Abaouz, A.; Journal of Solid State Chemistry 96 (1992) 324–331; doi:10.1016/S0022-4596(05)80266-X

data_1545896
_publ_section_title
;
 Crystal chemistry of anion-excess ReO3-related phases : crystal structure
 of beta-PrZr3F15
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              324
_journal_page_last               331
_journal_paper_doi               10.1016/S0022-4596(05)80266-X
_journal_volume                  96
_journal_year                    1992
_chemical_formula_sum            'F15 Pr Zr3'
_chemical_formula_weight         699.57
_space_group_IT_number           160
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                120.
_cell_formula_units_Z            3
_cell_length_a                   12.316(8)
_cell_length_b                   12.316(8)
_cell_length_c                   6.115(4)
_cell_volume                     803.3(9)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    7.500
_exptl_crystal_density_diffrn    4.34
_exptl_crystal_density_meas      4.36
_exptl_crystal_F_000             942
_refine_ls_number_parameters     36
_refine_ls_number_reflns         445
_refine_ls_R_factor_gt           0.033
_refine_ls_wR_factor_gt          0.033
_cod_data_source_file            JSSC-1992-96-324-331.cif
_cod_data_source_block           beta-PrZr3F15
_cod_original_cell_volume        803.3(13)
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_database_code               1545896
Synthesis and Characterization of [NH3(CH2)4NH3][Ga(PO4)(PO3OH)], a One-Dimensional Gallophosphate
Ann M. Chippindale; Andrew D. Bond; Ashley D. Law; Andrew R. Cowley; Journal of Solid State Chemistry 136 (1998) 227–232; doi:10.1006/jssc.1997.7685

data_1545897
_publ_section_title
;
 Synthesis and Characterization of [NH3(CH2)4NH3][Ga(PO4)(PO3OH)], a
 One-Dimensional Gallophosphate
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              227
_journal_page_last               232
_journal_paper_doi               10.1006/jssc.1997.7685
_journal_volume                  136
_journal_year                    1998
_chemical_formula_moiety         'Ga H O8 P2, 2(C2 H7 N)'
_chemical_formula_sum            'C4 H15 Ga N2 O8 P2'
_chemical_formula_weight         350.84
_space_group_IT_number           56
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      56
_symmetry_space_group_name_Hall  '-P 2ac 2bc'
_symmetry_space_group_name_H-M   'P n a a'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            4
_cell_length_a                   9.109(1)
_cell_length_b                   11.021(1)
_cell_length_c                   11.987(1)
_cell_volume                     1203.4(2)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.5418
_exptl_absorpt_coefficient_mu    14.19
_exptl_crystal_density_diffrn    1.936
_exptl_crystal_F_000             712
_refine_ls_number_parameters     100
_refine_ls_number_reflns         937
_refine_ls_R_factor_gt           0.0284
_refine_ls_wR_factor_gt          0.0354
_cod_data_source_file            JSSC-1998-136-227-232.cif
_cod_data_source_block           '[NH3(CH2)4NH3][Ga(PO4)(PO3OH)]'
_cod_original_formula_sum        'H15 C4 Ga N2 O8 P2'
_cod_database_code               1545897
Sol-gel synthesis and characterization of a new four-layer K0.5Gd0.5Bi4Ti4O15 Aurivillius phase
Kumar, Sunil; To be published in Journal Of Materials Science- Materials in Electronics  () –; doi:

data_3000126
_publ_section_title
;
 Sol-gel synthesis and characterization of a new four-layer
 K0.5Gd0.5Bi4Ti4O15 Aurivillius phase
;
_journal_name_full
'To be published in Journal Of Materials Science- Materials in Electronics'
_chemical_formula_sum            'Bi4 Gd0.5 K0.5 O15 Ti4'
_chemical_name_mineral           KGBT
_symmetry_space_group_name_Hall  'A -2 2a'
_symmetry_space_group_name_H-M   'A 21 a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.42798(52)
_cell_length_b                   5.41821(41)
_cell_length_c                   41.2723(33)
_cell_volume                     1213.82(18)
_cod_database_code               3000126
_cod_hold_until_date             2017-09-28
X-ray powder diffraction as a tool for facing twins: the case of the monoclinic NbCoTe2 and TaCoTe2 phases
Jing Li; Frank McCulley; Susan L. McDonnell; Norberto Masciocchi; Davide M. Proserpio; Angelo Sironi; Inorganic Chemistry 32 (1993) 4829–4833; doi:10.1021/ic00074a029

data_4345766
_publ_section_title
;
 X-ray powder diffraction as a tool for facing twins: the case of the
 monoclinic NbCoTe2 and TaCoTe2 phases
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4829
_journal_page_last               4833
_journal_paper_doi               10.1021/ic00074a029
_journal_volume                  32
_journal_year                    1993
_chemical_formula_sum            'Co Ta Te2'
_chemical_formula_weight         495.08
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90.
_cell_angle_beta                 116.789(4)
_cell_angle_gamma                90.
_cell_formula_units_Z            4
_cell_length_a                   8.1524(6)
_cell_length_b                   6.2649(4)
_cell_length_c                   7.7945(5)
_cell_volume                     355.37(4)
_diffrn_ambient_temperature      298
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.5418
_exptl_absorpt_coefficient_mu    222.33
_exptl_crystal_density_diffrn    9.25
_exptl_crystal_F_000             816
_pd_proc_ls_prof_R_factor        0.120
_pd_proc_ls_prof_wR_factor       0.155
_refine_ls_R_I_factor            0.046
_cod_data_source_file            Inorg-Chem-1993-32-4829-4833-1.cif
_cod_data_source_block           TaCoTe2
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               4345766
X-ray powder diffraction as a tool for facing twins: the case of the monoclinic NbCoTe2 and TaCoTe2 phases
Jing Li; Frank McCulley; Susan L. McDonnell; Norberto Masciocchi; Davide M. Proserpio; Angelo Sironi; Inorganic Chemistry 32 (1993) 4829–4833; doi:10.1021/ic00074a029

data_4345767
_publ_section_title
;
 X-ray powder diffraction as a tool for facing twins: the case of the
 monoclinic NbCoTe2 and TaCoTe2 phases
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4829
_journal_page_last               4833
_journal_paper_doi               10.1021/ic00074a029
_journal_volume                  32
_journal_year                    1993
_chemical_formula_sum            'Co Nb Te2'
_chemical_formula_weight         407.04
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90.
_cell_angle_beta                 117.487(3)
_cell_angle_gamma                90.
_cell_formula_units_Z            4
_cell_length_a                   8.1612(4)
_cell_length_b                   6.2976(3)
_cell_length_c                   7.8518(4)
_cell_volume                     358.00(3)
_diffrn_ambient_temperature      298
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.5418
_exptl_absorpt_coefficient_mu    192.12
_exptl_crystal_density_diffrn    7.55
_exptl_crystal_F_000             688
_pd_proc_ls_prof_R_factor        0.122
_pd_proc_ls_prof_wR_factor       0.163
_refine_ls_R_I_factor            0.040
_cod_data_source_file            Inorg-Chem-1993-32-4829-4833-2.cif
_cod_data_source_block           NbCoTe2
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               4345767